General

Mechanical

Property | Temperature | Value | Condition | Related Standards | Comment |
---|---|---|---|---|---|

Bending Fatigue Strength | 60.0 MPa Show Material materials with Bending Fatigue Strength of 60.0 MPa | T1 | AA Standards | ||

Compressive modulus | 69.7 MPa Show Material materials with Compressive modulus of 69.7 MPa | T1 | |||

Elastic modulus | 69.0 GPa Show Material materials with Elastic modulus of 69.0 GPa | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | ||

69 GPa Show Material materials with Elastic modulus of 69 GPa | T1 | ||||

Elongation | 20.0 % Show Material materials with Elongation of 20.0 % | T1 | AA Standards | A50 | |

12.0 % Show Material materials with Elongation of 12.0 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | A50 | ||

10.0 % Show Material materials with Elongation of 10.0 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | A100 | ||

16.0 % Show Material materials with Elongation of 16.0 % | T1 | ||||

370 °C | 105 % Show Material materials with Elongation of 105 % | T1 | Elongation in 50 mm | ||

315 °C | 80 % Show Material materials with Elongation of 80 % | T1 | Elongation in 50 mm | ||

260 °C | 75 % Show Material materials with Elongation of 75 % | T1 | Elongation in 50 mm | ||

205 °C | 40 % Show Material materials with Elongation of 40 % | T1 | Elongation in 50 mm | ||

150 °C | 20 % Show Material materials with Elongation of 20 % | T1 | Elongation in 50 mm | ||

100 °C | 18 % Show Material materials with Elongation of 18 % | T1 | Elongation in 50 mm | ||

24 °C | 33 % Show Material materials with Elongation of 33 % | T1 | Elongation in 50 mm | ||

0 °C | 34 % Show Material materials with Elongation of 34 % | T1 | Elongation in 50 mm | ||

-80 °C | 36 % Show Material materials with Elongation of 36 % | T1 | Elongation in 50 mm | ||

-195 °C | 44 % Show Material materials with Elongation of 44 % | T1 | Elongation in 50 mm | ||

Fatigue strength | 62 MPa Show Material materials with Fatigue strength of 62 MPa | T1 | fo 5x10⁸ cycles | ||

Hardness, Brinell | 42.0 [-] Show Material materials with Hardness, Brinell of 42.0 [-] | T1 | AA Standards | ||

42.0 [-] Show Material materials with Hardness, Brinell of 42.0 [-] | T1 | 500 kg load, 10 mm ball | |||

Plane-Strain Fracture Toughnes | 22.0 - 35.0 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 22.0 - 35.0 MPa·√m | Typical for Wrought 6000 Series Aluminium | |||

Poisson's ratio | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | Typical for Wrought 6000 Series Aluminium | |||

Shear modulus | 26.0 - 26.5 GPa Show Material materials with Shear modulus of 26.0 - 26.5 GPa | Typical for Wrought 6000 Series Aluminium | |||

Shear strength | 97.0 MPa Show Material materials with Shear strength of 97.0 MPa | T1 | |||

Tensile strength | 150.0 MPa Show Material materials with Tensile strength of 150.0 MPa | T1 | AA Standards | ||

115.0 MPa Show Material materials with Tensile strength of 115.0 MPa | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | |||

110.0 MPa Show Material materials with Tensile strength of 110.0 MPa | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | |||

140.0 MPa Show Material materials with Tensile strength of 140.0 MPa | T1 | ||||

370 °C | 16 MPa Show Material materials with Tensile strength of 16 MPa | T1 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

315 °C | 22 MPa Show Material materials with Tensile strength of 22 MPa | T1 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

260 °C | 31 MPa Show Material materials with Tensile strength of 31 MPa | T1 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

205 °C | 62 MPa Show Material materials with Tensile strength of 62 MPa | T1 | |||

150 °C | 145 MPa Show Material materials with Tensile strength of 145 MPa | T1 | |||

100 °C, 24 °C | 152 MPa Show Material materials with Tensile strength of 152 MPa | T1 | |||

0 °C | 165 MPa Show Material materials with Tensile strength of 165 MPa | T1 | |||

-80 °C | 180 MPa Show Material materials with Tensile strength of 180 MPa | T1 | |||

-195 °C | 235 MPa Show Material materials with Tensile strength of 235 MPa | T1 | |||

Unlock all property charts | |||||

Yield strength | 90.0 MPa Show Material materials with Yield strength of 90.0 MPa | T1 | AA Standards | RP02 | |

60.0 MPa Show Material materials with Yield strength of 60.0 MPa | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | RP02 | ||

55.0 MPa Show Material materials with Yield strength of 55.0 MPa | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | RP02 | ||

371 °C | 14 MPa Show Material materials with Yield strength of 14 MPa | T1 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

316 °C | 17 MPa Show Material materials with Yield strength of 17 MPa | T1 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

260 °C | 24 MPa Show Material materials with Yield strength of 24 MPa | T1 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

204 °C | 45 MPa Show Material materials with Yield strength of 45 MPa | T1 | |||

149 °C, -80 °C | 103 MPa Show Material materials with Yield strength of 103 MPa | T1 | |||

100 °C, -28 °C | 97 MPa Show Material materials with Yield strength of 97 MPa | T1 | |||

24 °C | 90 MPa Show Material materials with Yield strength of 90 MPa | T1 | |||

-196 °C | 110 MPa Show Material materials with Yield strength of 110 MPa | T1 | |||

78.0 MPa Show Material materials with Yield strength of 78.0 MPa | T1 | ||||

Unlock all property charts |

Thermal

Property | Temperature | Value | Condition | Related Standards |
---|---|---|---|---|

Coefficient of thermal expansion | 2.3e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3e-05 1/K | T1 | ||

100 °C, 20 °C | 2.3399999999999996e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3399999999999996e-05 1/K | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | |

Melting point | 615.0 - 655.0 °C Show Material materials with Melting point of 615.0 - 655.0 °C | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | |

620.0 °C Show Material materials with Melting point of 620.0 °C | T1 | |||

Specific heat capacity | 900.0 J/(kg·K) Show Material materials with Specific heat capacity of 900.0 J/(kg·K) | T1 | ||

Thermal conductivity | 193.0 - 218.0 W/(m·K) Show Material materials with Thermal conductivity of 193.0 - 218.0 W/(m·K) | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | |

200.0 W/(m·K) Show Material materials with Thermal conductivity of 200.0 W/(m·K) | T1 |

Electrical

Property | Value | Condition | Related Standards | Comment |
---|---|---|---|---|

Electrical conductivity | 29000000.0 - 34000000.0 S/m Show Material materials with Electrical conductivity of 29000000.0 - 34000000.0 S/m | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | |

29000000 S/m Show Material materials with Electrical conductivity of 29000000 S/m | T1 | Typical value | ||

Electrical resistivity | 2.94e-08 - 3.45e-08 Ω·m Show Material materials with Electrical resistivity of 2.94e-08 - 3.45e-08 Ω·m | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 | |

3.4e-08 Ω·m Show Material materials with Electrical resistivity of 3.4e-08 Ω·m | T1 | Typical value | ||

Specific Electrical conductivity | 50.0 % IACS Show Material materials with Specific Electrical conductivity of 50.0 % IACS | T1 | Typical/Derived value |

Chemical properties

Property | Value | Condition | Related Standards |
---|---|---|---|

Aluminium | 97.5 - 99.4 % Show Material materials with Aluminium of 97.5 - 99.4 % | T1 | |

Chromium | 0.1 % Show Material materials with Chromium of 0.1 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 |

Copper | 0.1 % Show Material materials with Copper of 0.1 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 |

Iron | 0.35 % Show Material materials with Iron of 0.35 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 |

0.35 % Show Material materials with Iron of 0.35 % | T1 | ||

Magnesium | 0.45 - 0.9 % Show Material materials with Magnesium of 0.45 - 0.9 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 |

Manganese | 0.1 % Show Material materials with Manganese of 0.1 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 |

Other | 0.15 % Show Material materials with Other of 0.15 % | T1 | |

Silicon | 0.2 - 0.6 % Show Material materials with Silicon of 0.2 - 0.6 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 |

Titanium | 0.1 % Show Material materials with Titanium of 0.1 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 |

Zinc | 0.1 % Show Material materials with Zinc of 0.1 % | T1 | AA Standards, ASTM B221, ASTM B241, ASTM B345 |

Technological properties

Property | ||
---|---|---|

Brazing | general: possible with commercial processes and methods | |

Corrosion properties | Stress corrosion cracking: no damage during operation and laboratory tests, general: very good, without protection in industrial or seawater atmosphere | |

General machinability | General: poor (T1, T4), sufficient (T5, T452, T6, T83, T831, T832) | |

Workability | general (condition): acceptable (T1, T4, T5, T452), poor(T6, T83, T831, T832) |